doi:10.5368/aedj.2011.3.4.1.5THE EFFECT OF FLOWABLE COMPOSITE LINING THICKNESS WITH VARIOUS CURING TECHNIQUES ON INTERNAL VOIDS IN CLASS II COMPOSITE RESTORATIONS-AN INVITRO STUDY. ^ Nagalakshmi Reddy S Reader ^Baiju Gopalan Nair Professor and Head ^ Amarendher reddy.k Professor * pratap kumar.M Professor ^Samba Shiva rao Reader^^^ Department of Conservative Dentistry and Endodontics ,G.Pulla Reddy Dental College, Kurnool , Andhra Pradesh, India.•^ Department of Conservative Dentistry and Endodontics, Meghana institute of Dental sciences, Mallaramvillage, nizamabad, Andhra Pradesh, India.ABSTRACT:Aim of this studv was to compare class II composite restoration using flowable composites as lininq with various thickness andcuring techniques by evaluating internal voids. Fifty intact molars, each prepared with two box-only class II cavities, wererandomly divided into five groups: Group I, P 60 filling alone; Group II, ultra thin flowable composite lining (0.5-1 mm) co-curedwith overlying composite; Group III, thin lininq (1-1.5) co-cured with overlyinq composite; Group IV, ultra thin lininq (0.5-1 mm)precured and Group V, thin lining (1-1.5) precured. Internal voids were recorded in the gingival interface, cervical and occlusalhalves of restorations. Precured techniques for flowable composite lining showed the least number of interface and cervicalvoids where as the co-cured technique of flowable and packable composites showed the least number of occlusal voids.KEY WORDS: Packable composite; flowable composite; precure technique; co-cure technique; ultra thinlining and thin lining.INTRODUCTION Packable composite was developed by changing the Methodologyfiller or matrix phase to increase viscosity for better Freshly extracted fifty human molars were mountedcondensation similar to that of amalgam. However ability on dental stone with one premolar and one molar on theto adequately adapt the internal areas was always mesial and distal sides to simulate posterior toothquestionable^. So in an attempt to reduce the voids, alignment and were prepared with standardized mesiovarious incremental techniques, curing techniques and occlusal and disto occlusal box only class II cavitieslining materials have been designed Flowable having bucco-lingual width 4 mm, mesio distal width 2mmcomposites were introduced in late 1996. They are non- and occluso gingival depth of 3 mm. Sectional matrix bandsticky and injectable. They have low viscosity and was placed which was stabilized with G-rings and woodenincreased wettability due to lower filler contend. Flowable wedges. They were etched with 35% phosphoric acid,composite as a lining material for class II resin composites washed thoroughly with water for 15 seconds and followedreduced voids*. Considering the advantages and by the application of the two layers of single bond anddisadvantages of various types of composites and each layer was cured with curing light for 10 seconds. Thetechniques, recently a new technique was introduced by 50 molar teeth were randomly divided into 5 groups of 10Jackson and Morgan 2000 where a thin layer of flowable teeth each. Group I: Cavity preparations were restoredcomposite is applied to cavity floor which is immediately with posterior composite alone .e.Pm, Group II: Cavityfollowed by packable composite increment and light cured. preparations were lined with flowable composite (FiltekMost of flowable composite is expelled while placing flow) to about 0.5-1 mm occluso gingival thickness, thenoverlying composite and its volume will be minimized. This 1mm thick posterior composite (P6o) was insertedtechnique offers the advantage of two different composites immediately and cured together (co cured). Group III: Itincluding intimate adaptation of filling and handling was similar to group II except lining thickness was 1-properties^. Accordingly this invitro study compared class 1.5mm, Group IV: Cavity preparations were lined withII composite restorations using flowable composite lining ultra thin layer of flowable composite i.e. 0.5-1 mm andeither with the modified incremental technique or with cured for 20 seconds (precured). Remaining cavity wasvarious thicknesses by evaluating internal voids. filled with posterior composite. Group V: It was similar toVollll. Issue 4 Oct-Dec 2011 22
Table.1 Interface voids rating Graph.1. Interface voids pattern Interface Groups No. Voids - Voids + Grapli 1 : mtertace Voids Pattern Gr. 1 40 21 (52.5) 19(47.5) Gr. II 40 34 (85) 6(15) Gr. Ill 40 32 (80) 8(20) 40 Gr. IV 40 40(100) 0 Gr. V 40 40(100) 0 Gr. Ml t = 9.83 P = 0.01,S Gr. Nil )i = 6.77 P = 0.01,S 0 Interface VOIDS o Gr. I-IV )f^ = 24.91 P = 0.001, HS a Interf ace VOIDS 1 Gr. I-V t = 24.91 P = 0.001, HS Comparison Gr. IHII ï = 0.35 P = 0.56, NS between Gr. II-IV y = 6.49 P = 0.05, S groups Gr. Il-V y = 6.49 P = 0.05, S n Gr. III-IV ¡r = 8.89 P = 0.01,S Grl Gril •>[ I v l.? • Gr. Ill-V t = 8.89 P = 0.01,S Gr. IV-V ir= 0.00 P = 1.00, NS Table.2 cervical voids rating Cervical Graph.2. Cervical voids pattern Groups No. Voids - Voids + Gr. 1 40 4(10) 36 (90) Graph 2 : Cervical Voids Patttm Gr. II 40 10(2.5) 30 (75) Gr. Ill 40 8(20) 32 (80) 10 -, Gr. IV 40 13(32.5) 27 (67.5) 35 - Gr. V 40 18 (45) 22 (55) Gr. NI li = 3.11 P = 0.08, NS 25 • Gr. Nil )c = 1.57 P = 0.21,NS 20 - nCervtcal VOIDS 0 Gr. I-IV y = 6.05 P = 0.05, S t5 • DCeivical VOIDS 1 n Gr. I-V y = 12.3 P = < 0.05, S 10 - Comparison Gr. IHII 1 = 0.29 P = 0.59, NS between 5- groups Gr. II-IV y = 0.55 P = 0.46, NS 0 Gr. Il-V y = 3.52 P = 0.06, NS Gr I Gr II Gt III CM- IV Gr Gr. IIHV y.= 1.61 P = 0.20, NS Gr. Ill-V r} = 5.70 P = 0.05, S Gr. IV-V y = 1.32 P = 0.25, NS Table.3 . Occlusal voids rating Graph.3. Occlusal voids pattern Groups Occlusal NO. Voids - Voids + Gr. 1 40 4(10) 36 (90) Graph 3 : Occlusal Voldi Pittarn Gr. II 40 8(20) 32 (80) 40 Gr. Ill 40 7(17.5) 33 (82.5) Gr. IV 40 5 (12.5) 35 (87.5) 3S Gr. V 40 6(15) 34 (85) 30 • n n Gr. l-ll y.^=1.57 P = 0.21,NS Gr. l-lll X = 0.95 P = 0.33, NS 20 • OccluMI VOIDS 0 Qcclusal VOIDS I Gr. NV y^ = 0.13 P = 0.72, NS 15 • Gr. I-V )f. = 0.46 P = 0.50, NS 1 Comparison Gr. ll-lll 10 • x = 0.08 P = 0.77, NS between 6- groups Gr. II-IV y = 0.83 P = 0.36, NS 0 Gr. Il-V I = 0.35 P = 0.56, NS Grl GrII Ql Ul Si IV Gr. III-IV )( = 0.39 P = 0.53, NS Gr. Ill-V y = 0.09 P = 0.76, NS Gr. IV-V y = 0.10 P = 0.74, NSVol III. Issue 4 Oct- Dec 2011 23
group IV except lining thickness was 1-1.5mm. The conducted to compare class II composite restoration usingrestorations were cured via buccal and lingual aspects for flowable composites as lining with various thickness and20 seconds. They were mesio-distally sectioned using a curing techniques by evaluating the internal voids.hard tissue microtome and were examined under a 50xstereomicroscope. In Internal voids evaluation voids were The result of the present study reveals that internalseen in three sites - Occlusal half of restorations. Cervical voids predominantly consisted of interface and cervicalhalf of restorations. Gingival interface (restorative interface voids (Tabie-I and Table II). Group I showed highof cervical margin). Voids were scored as follows: No prevalence of interface and cervical voids (Graph-1 & 2 ) .voids = 0, Visible voids = 1. Group wise comparisons are The presence of such voids may contribute to deficientmade by Mann-Whitney test. Categorical data are cavity adaptation and unavoidable trapping of air whileanalyzed by Chi-square test. For all the tests a p-value of manipulating a posterior composite. Group II results0.05 or less was considered for statistical significance. indicated that the incidence of interface and cervical voids decreased when compared to Group I, with the applicationResults: of flowable linings, but remained higher than the precured groups (Group-IV&V). The results of the present study arePrecured specimens showed less number of voids and in agreement with a study conducted to evaluate thecontrol specimens showed maximum number of voids. In microleakage and internal voids in class II compositeinterface and cervical half on comparison of curing restorations with flowable composite lining (precured)techniques, precured specimens showed less number of showed a reduction in the number of voids as compared tovoids than co-cured specimens. (Table-I and Table II). In those in which flowable lining was usecf.Packing theocclusal half on comparison of curing techniques, co- composite may cause incorporation of air. A studycured specimens showed less number of voids than conducted to evaluate the incidence of interface voids andprecured specimens. (Table-Ill). In interface and cervical microleakage of class II box only composite restorationhalf on comparison of lining thickness and type of curing. with ultra thin flowable resin lining showed moderateGroup IV showed less number of voids than Group V. incidence of interface voids^. A study conducted to(Table - 2). In occlusal half on comparison of lining evaluate effect of flowable resin composite onthickness and type of curing. Group V showed less microleakage and interface voids in class II compositenumber of voids than Group IV. Group II showed less restorations revealed reduced interface voids and totalnumber of voids than Group III in interface and occlusal number of voids were reduced in restoration^ .This is duehalf. (Graph-1 and 3) Group III showed less number of to enhanced cavity adaptation, low modulus of elasticity,voids than Group II in cervical half. (Grapii-2). increased wetting of flowable composites and there by leading to lesser number of voids*.Discussion The results of the present study are in agreement with With increased patient interest in esthetic alternatives another study which evaluated shrinkage stress reductionto dental amalgam, the objectives were to modify the on porosity concentration in thin resin layers. This studyhandling characteristics of RBC". Voids are usually demonstrated that reduced contraction stresses could beproduced by the air trapped during mixing or application obtained by using a thin, pore containing lining material.procedures. It is based on free radical polymerization and Both the presence of minimal voids and setting inhibitioncontains redox system which promotes bulk effect caused by the oxygen present in these voids couldpolymerization inhibition due to high chemical affinity of provide relief polymerization stress and result in reducedatmospheric oxygen for free radicals. It creates surface microleakage. The study also suggests that care must bediscontinuities, which increases fracture propagation and taken not to trap air during placement of flowablefailure on loading. Poor marginal adaptation is related to composite. The repeated packing motion followinginternal voids. Larger voids will reduce the mechanical placement of overlying composite must be avoided tostrength of restoration®. To reduce the internal voids, prevent undue porosity formation^.flowable composites are used as a liner and cured, overwhich the final packable composite is placed and curedincrementally which was suggested as a precured method From the results of the present study it can beof placement^ A study conducted to evaluate the effect of concluded that the co-cured flowable lining compositeflowable composite lining on microleakage and internal restorations showed greater internal voids when comparedvoids in class II composite restorations revealed few to precured flowable lining composite restoration.cervical voids in flowable lining restorations. Nowrecently, in a new technique called co-cured technique, a CONCLUSIONthin layer of flowable composite is applied to the cavityfloor which is immediately followed by packable composite An ultra thin lining of flowable composite at the baseincrement and then light cured together. This technique of the cavity followed by precuring technique and then theoffers the advantage of intimate adaptation of filling and incremental build up of packable composite showed theimproved handling properties^. The present study was least number of interface voids. A thin lining of flowableVol ill. Issue 4 Oct- Dec 2011 24
Fig.1. Schematic representation of class II box only cavity Fig.3. Class II box preparation ( MO and DO) preparation Fjg.2. Specimens used in the study Fig.4. Specimen after sectioning with microtome Fig.5. Specimen showing internal voidsVollll. Issue 4 Oct-Dec 2011 25
composite at the base of the cavity followed by precuring Corresponding Authortechnique and then the incremental build up of packablecomposite showed the least number of cervical voids. An Dr.Nagalakshmi Reddyultra thin lining of flowable composite at the base of the Department of conservative Dentistrycavity followed by co-curing technique of both the flowable G.pulla Reddy Dental college and Hospitaland packable composite showed the least number ofocclusal voids. Nandhyala road KURNOOL-518003References PH:273360 Mobile:9490197767 1. Chuang SF, Liu JK. Effects of flowable composite Email:lakshnni_reddy61 @ yahoo.com. lining and operative experience on microleakage and internal voids in class II composite restorations. J Prosthet dent 2001 ;85:177-83. PMid: 11208208 http://dx.d0i.0rg/i 0.1067/mpr.2001.113780 2. Leevailoj C. Cochran MA, Matis BA, Moore BK, Plate JA. Microleakage of posterior packable resin composite with and without flowable liners Oper Dent 2001;26:302-307. PMid: 11357574 3. Malmstrom H. Schlueter M, Roach T, Moss ME. Effective thickness of flowable resins on marginal leakage in class II composite restorations. Oper Dent 2002;27:373-380. PMid:12120775 4. Estafan D, Estafan A, Leinfelder K. Cavity wall adapatation of resin based composites lined with flowable composites. J Am Dent 2000;13(4):192-194. 5. Chuang SF, Tin YT, Liu JK, Chang CH, Shieh DB. Influence of flowable composite lining thickness on class II composite restorations. Oper Dent 2004; 29(3):301-308. PMid:15195731 6. Chuang SF, Liu JK, Jin YT. Microleakage and internal voids in Class II composite restorations with flowable composite linings. Operative Dentistry 2001;26:193- 200. 7. KorkmazY, Ozel E, Attar N. Effect of flowable composite lining on microleakage and intemal voids in classll composite restorations. Journal of Adhes Dent 2OO7;9(2):189-194. 8. Olmez A, Oztas N, Bodur H. The effect of flowable resin composite on microleakage and internal voids in class II composite restorations. Oper Dent 2004;29(6):713-719. PMid:15646229 9. Alster D, Feilzer AJ, de Gee AJ, Mor A, Davidson CL The dependence of shrinkage stress reduction of porosity concentration in thin resin layers. Journal of Dental Res 1992;71(9):1619-1622. PMid:1522296 http://dx.doi.Ofa/10.1177/00220345920710091401Vollll. Issue 4 Oct-Dec 2011 26
Copyright of Annals & Essences of Dentistry is the property of Dentaquest and its content may not be copied oremailed to multiple sites or posted to a listserv without the copyright holders express written permission.However, users may print, download, or email articles for individual use.